Photoinduced oxygen release and persistent photoconductivity in ZnO nanowires
© Bao et al; licensee Springer. 2011
Received: 17 January 2011
Accepted: 31 May 2011
Published: 31 May 2011
Photoconductivity is studied in individual ZnO nanowires. Under ultraviolet (UV) illumination, the induced photocurrents are observed to persist both in air and in vacuum. Their dependence on UV intensity in air is explained by means of photoinduced surface depletion depth decrease caused by oxygen desorption induced by photogenerated holes. The observed photoresponse is much greater in vacuum and proceeds beyond the air photoresponse at a much slower rate of increase. After reaching a maximum, it typically persists indefinitely, as long as good vacuum is maintained. Once vacuum is broken and air is let in, the photocurrent quickly decays down to the typical air-photoresponse values. The extra photoconductivity in vacuum is explained by desorption of adsorbed surface oxygen which is readily pumped out, followed by a further slower desorption of lattice oxygen, resulting in a Zn-rich surface of increased conductivity. The adsorption-desorption balance is fully recovered after the ZnO surface is exposed to air, which suggests that under UV illumination, the ZnO surface is actively "breathing" oxygen, a process that is further enhanced in nanowires by their high surface to volume ratio.
Semiconductor nanowires provide a natural, ready-made structure in applications where small dimensions are required [1–3]. Their small diameter (≤100 nm) implies that a host of surface effects can influence their electrical and optical properties, which is important for the functionality and performance of nanowire-based devices [4–6]. Some observations such as enhanced gas sensitivity and photoconductivity, nowadays reconfirmed in ZnO nanowires [7–11], have been known in ZnO whiskers and thin films, and several attempts have been made to explain their occurrence [12–14]. The element, proposed here to tie together the various pieces of the puzzle into a single comprehensive model, is a fully reversible carbon-catalyzed photolysis, where carbon is omnipresent due to the pervasiveness of surface hydrocarbons, capable of exposing zinc on ZnO surfaces upon ultraviolet (UV) exposure. This surface effect is more pronounced and easily observed in structures of high surface-to-volume ratio, such as nanowires.
ZnO is a wide bandgap semiconductor material that has been attracting considerable research interest for many years. It has recently seen a renaissance due to reports of successful p-type doping , room-temperature ferromagnetism which could make it attractive for spintronic devices , and the large exciton binding energy which makes it attractive for photonics . ZnO nanowire applications such as lasers, light-emitting diodes, nanogenerators, and field emitters have been reported [18–21]. In most of these applications, the typical surface sensitivity of the nanowire structure is often a disadvantage. However, ZnO nanowires are also finding use as gas sensors and UV detectors [7–11, 22]. These nanowire sensors make use of the known surface sensitivity of ZnO which is further enhanced by the nanowire structure. The nature of this sensitivity has been controversial for over half a century [12–14, 23, 24]. Nanowires provide a new opportunity to look at the underlying mechanism of this surface sensitivity, which is the purpose of this work.
It has been known for many years that when ZnO films are exposed to above-bandgap (UV) illumination, their conductivity increases rapidly but persists long after the UV light is turned off . This persistence has been shown to depend on the availability of ambient oxygen and has led to the suggestion of surface electron depletion region tightly related to the surface density of negatively charged adsorbed oxygen species ( ) . UV light causes this loosely bound oxygen to desorb from the surface at an increased rate, shifting the balance from adsorption to desorption. This reduces the surface electron depletion region leading to enhanced photoconductivity.
In vacuum, desorbed oxygen is pumped away. Therefore, this state of oxygen depletion may persist for as long as good vacuum is maintained. The density of these loose species of surface oxygen may be totally eliminated in vacuum, and therefore, one may expect under the same UV photon flux a somewhat higher conductivity to be reached in vacuum compared with that in air. The common observation is, however, of a much larger increase [7–11]. As we here report, the rate of photocurrent increase in ZnO nanowires associated with oxygen desorption in vacuum shows in fact two processes: one fast at a rate comparable to that in air and another one much slower that continues long after the first process has ended.
In the pioneering study on ZnO whiskers by Collins and Thomas , it was argued that the disappearance of the depletion region in vacuum alone cannot account for the large increase in conductivity and that a Zn-rich conductive layer, created by surface photolysis of lattice oxygen, was responsible for the large increase in photoconductivity observed in vacuum . The large surface-to-volume ratio in the nanowire structure should enhance this effect, and indeed, several recent studies on ZnO nanowires have pointed out such increased photocurrent in vacuum [7–11].
In this work, we investigated photoconductivity of ZnO single nanowires in air and vacuum, and we found that the photoconductivity is much larger in vacuum than in air. We argued that this much enhanced photoconductivity arises from the decomposition of ZnO - surface photolysis of ZnO, and it cannot be explained by simple desorption of absorbed oxygen species. We further proposed that the ZnO photolysis is photocatalyzed by surface carbon, giving rise to the release of oxygen species in the form of carbon dioxide.
ZnO nanowires in this study were synthesized by chemical vapor deposition using the vapor-liquid-solid technique . Carbothermally reduced ZnO was used as the source material, and the gold nanoparticles were used as catalyst to seed and control the growth on a silicon substrate. Crystalline quality was assessed using transmission electron microscopy (TEM). ZnO nanowire photoconductors were prepared on an oxidized Si wafer with a 1-μm-thick silicon dioxide insulating layer. Electrical contacts were defined by electron-beam lithography and lift-off. They consisted of 5-nm thick of titanium and 50-nm thick of gold deposited sequentially using thermal evaporation. To achieve ohmic characteristics, the devices were then thermally treated for 10 min at 400°C in a mixed gas of 5% hydrogen and 95% helium at a total flow rate of 200 sccm.
Photoluminescence was excited using the 325-nm line of a He-Cd laser. Photoconductivity measurements were carried out at room temperature in a quartz-window optical cryostat, which can be filled with air or pumped to a vacuum of less than 10-5 Torr. A high-pressure mercury lamp was used as a UV light source, and a bandpass filter (313-nm center wavelength, 10-nm bandwidth) was used to obtain monochromatic UV light from the mercury lamp.
Results and discussion
Persistent photoconductivity in ZnO has been observed in most of its known structures: thin films, microneedles, and nanowires (except, of course, for quantum dots because at least one dimension is required for conduction) [10, 12, 14, 22]. Besides, by release of trapped electrons, carriers are also created through photogeneration of electron-hole pairs. To obtain an upper limit for this contribution, we note that the ZnO absorption length for light at 313 nm is comparable to the wire diameter (approximately 100 nm) and assume that all of the incident light is absorbed. Since ZnO is a direct bandgap semiconductor, the lifetime of photogenerated electron-hole pairs is shorter than 1 ns [26, 27]. Taking for the lifetime 1 ns and assuming for the UV intensity the experimental value of ≈3.0 mW/cm2, the generated electron density is approximately 5 × 1011/cm3, and the corresponding photocurrent at 0.3 V bias voltage across the approximately 1.8 μm distance between two electrodes (see Figure 1) is about 2.5 × 10-4 nA, assuming an electron mobility of approximately 20 cm2/Vs [9, 10]. This current is about six orders of magnitude less than the dark current we observed. Optically excited carriers may decay into excitons which have a longer lifetime, but excitons do not contribute to the photoconductivity due to the charge neutrality. We therefore may safely neglect the contribution of photogenerated free carriers to the photocurrent in our case of weak illumination.
Undoped ZnO typically shows n-type conductivity, often suggested to be related to oxygen vacancies [7, 9, 10, 12, 28]. However, first-principles calculations showed that oxygen vacancies are not a shallow donor but rather a deep level . Oxygen vacancies are more likely to be found close to surfaces, especially in the case of nanowires, and thereby to serve as surface traps [9, 10, 28, 30, 31].
Trapping of electrons charges the surface negatively, creating a non-conducting depletion layer under the surface. As previously discussed, a decrease or disappearance of this depletion layer under UV illumination underlies the photoconductivity of Zn nanowires. In the dark, reducing the oxygen pressure has only a minor effect on the adsorbed oxygen. This is evident in the rather minor change of conduction in vacuum from that in air prior to UV exposure, as shown in Figure 1.
As the illumination is turned off, adsorbed oxygen molecules trap electrons, gradually bending the bands, raising the surface potential barrier and the internal field. This reduces electron trapping at the surface, thereby reducing oxygen adsorption, and promotes spatial separation of electrons and photogenerated holes, thereby increasing their recombination lifetime. This positive feedback cycle qualitatively explains the persistence and non-exponential decay of the photocurrent as shown in Figures 2, 3, and 4.
In air, the discharging of the oxygen-related surface states and the resulting desorption of oxygen, as well as the shrinking of the depletion layer, require about 2 to 3 min, under UV illumination intensity on the order of 1 mW/cm2, as indicated by the time the photocurrent takes to reach its steady-state value. In vacuum, we basically have the same process, and therefore, it should be expected to take a roughly similar duration to establish a steady state. Of course, in vacuum, the steady state should be different, as there is no equilibrium between desorbed and adsorbed oxygen. Oxygen desorbs in vacuum at the same rate as in air, but since the oxygen is readily pumped out, it cannot be re-adsorbed . Thus, the surface oxygen can be totally desorbed, totally eliminating the contribution of the adsorbed oxygen to the depletion and band bending. Indeed, in vacuum, we observe an initial rapid rise in the photoconductivity that reaches somewhat beyond the value reached in air (it rises to about 0.5 μA in the first 2 to 3 min). However, this transient is followed by a slower rise that continues for few hours and cannot be accounted for by the rapid process, in which loosely bound oxygen is desorbed. What could then explain this additional slow rise in vacuum?
To account for the slow response, we first note that this vacuum photoconductivity is not observed to saturate, even after hours of exposure, while in air, saturation is reached relatively fast, and that both air and vacuum photoconductivities are fully reversed upon exposure to oxygen in the dark. This suggests that the second, slower photoconductivity increase that we observe in vacuum is related to oxygen desorption as well. However, the slow and prolonged nature of this second process suggests that this oxygen is more tightly bound. Could it be lattice oxygen?
The idea of lattice oxygen desorption in ZnO was put forth to explain photoconductivity in whiskers . It was suggested that the photoexcited holes, responsible for desorption of what we denote as loosely bound oxygen, are also responsible for subsequent lattice decomposition. This idea has not received enough attention since it is difficult to imagine that excess holes alone would be enough to decompose a lattice, held together by the high cohesive energy typical of oxide crystals. Nonetheless to date, several other stable materials, e.g., CdS, have been reported to show a so-called surface photolysis, where the anion was observed to be released upon exposure to above-bandgap illumination . The question is therefore: why would such a process occur in ZnO?
Shapira et al. used mass spectrometry and Auger electron spectroscopy to identify the species desorbed from ZnO upon exposure to UV illumination in vacuum, as in our experiment . They found that oxygen is desorbed from the surface of ZnO in the form of CO2 and suggested that surface hydrocarbons, commonly present on many solid surfaces, work in conjunction with the incident photon energy to release oxygen from the ZnO lattice, in a process that may be reversed by exposure to gaseous oxygen in the dark. Today, carbon is known to reduce oxides in what has been dubbed "carbothermal reduction" . Carbothermal reduction is commonly used to enable decomposition of oxides at temperatures lower than their typical decomposition temperature, e.g., in ZnO nanowire growth . It is therefore possible that if one changes the energy source from thermal to optical, carbon may still enhance oxide decomposition. In other words, we propose that when carbon is present on the surface, a "carbo-optical" reaction may be responsible for the slow oxygen desorption process we observe under UV exposure in vacuum.
We note, however, that although hydrocarbons are almost always present, it is not absolutely clear whether the presence of carbon is critical for ZnO photolysis, as there has also been a single report of O2 photodesorption from ZnO . We also note that it may be possible that oxygen containing compounds other than O2, e.g., H2O, could serve as oxygen source to replenish the lost oxygen , although CO2 was clearly found ineffective . Nonetheless, it is clear that only oxygen can take the place of the lost lattice oxygen and restore the resistivity, regardless of the actual chemical species supplying it. Finally, it was proposed that two electron-hole (excitons) pairs could provide enough energy to photodecompose lattice ZnO . However, firstly, this model is partial as it does not require carbon, and if it actually worked, we should be able to detect emission of oxygen, while in fact it is CO2 that is actually detected. Secondly, a process requiring two electron-hole pairs to be perfectly timed to act together as one is of very low probability, if at all possible. On the other hand, the same process involving carbon, as we propose, should require less energy and would easily account for the observed CO2 emission.
Free electrons released from desorbed oxygen, as well as from the Zn-rich surface layer, should remain free as long as the ZnO nanowire is maintained in perfect vacuum, leading to indefinitely persistent photoconductivity. The minor decay of photocurrent we observe in vacuum clearly reflects the residual oxygen and is thus a rough indicator of our vacuum quality.
where ε is the permittivity of ZnO (ε is approximately 8.5) . Assuming ϕ = 1.15 V, as previously suggested, we obtain d crit ≈ 100 nm. This value is about the actual diameter of the ZnO nanowire. The nanowire is then likely to be near total depletion, in agreement with its low dark conductivity.
In summary, we proposed a model to account for the observed persistent photoconductivity in ZnO nanowires, which ties together several previously suggested explanations of different facets of the problem into a single comprehensive picture. Negatively charged traps associated with adsorbed oxygen deplete ZnO nanowires of electrons. This oxygen-related depletion is partially undone by exposure to UV in air and completely reversed by UV exposure in vacuum. UV exposure in air removes loosely bound oxygen and in vacuum further removes lattice oxygen in a process that may be catalyzed by surface hydrocarbons. According to the suggested model, carbon-catalyzed photolysis is responsible for the slow release of lattice oxygen, exposing zinc on ZnO surfaces upon UV exposure in vacuum or low oxygen environment. This effect is more pronounced in structures of high surface-to-volume ratio like nanowires. This oxygen removal, however, is fully reversible upon exposure to oxygen in the dark, in a process that is somewhat reminiscent of breathing. We note that the role of loosely bound oxygen in inducing electron surface traps could possibly be assumed by oxygen containing molecules, e.g., water, which could also serve to reverse the slow photolysis taking place in vacuum.
JMB thanks Dr. Jie Xiang for help with E-beam lithography, and Mariano Zimmler and Professor Carsten Ronning for many valuable discussions. JMB also acknowledges support from TcSUH of the University of Houston and the Robert A. Welch Foundation (E-1728). I. Shalish thanks Professor Yoram Shapira for helpful discussions and acknowledges a Converging Technologies personal grant from the Israeli Science Foundation - VATAT. The work performed at Boston College is supported by DOE DE-FG02-00ER45805 (ZFR).
- Lieber CM: Nanoscale science and technology: building a big future from small things. Mrs Bulletin 2003, 28: 486–491. 10.1557/mrs2003.144View Article
- Huang Y, Lieber CM: Integrated nanoscale electronics and optoelectronics: exploring nanoscale science and technology through semiconductor nanowires. Pure and Applied Chemistry 2004, 76: 2051–2068. 10.1351/pac200476122051View Article
- Samuelson L, Thelander C, Bjork MT, Borgstrom M, Deppert K, Dick KA, Hansen AE, Martensson T, Panev N, Persson AI, Seifert W, Sköld N, Larsson MW, Wallenberg LR: Semiconductor nanowires for 0D and 1D physics and applications. Physica E-Low-Dimensional Systems & Nanostructures 2004, 25: 313–318. 10.1016/j.physe.2004.06.030View Article
- Wang DW, Chang YL, Wang Q, Cao J, Farmer DB, Gordon RG, Dai HJ: Surface chemistry and electrical properties of germanium nanowires. Journal of the American Chemical Society 2004, 126: 11602–11611. 10.1021/ja047435xView Article
- Shalish I, Temkin H, Narayanamurti V: Size-dependent surface luminescence in ZnO nanowires. Physical Review B 2004, 69: 245401.View Article
- Calarco R, Marso M, Richter T, Aykanat AI, Meijers R, Hart AV, Stoica T, Luth H: Size-dependent photoconductivity in MBE-grown GaN-nanowires. Nano Letters 2005, 5: 981–984. 10.1021/nl0500306View Article
- Kind H, Yan HQ, Messer B, Law M, Yang PD: Nanowire ultraviolet photodetectors and optical switches. Advanced Materials 2002, 14: 158. 10.1002/1521-4095(20020116)14:2<158::AID-ADMA158>3.0.CO;2-WView Article
- Soci C, Zhang A, Xiang B, Dayeh SA, Aplin DPR, Park J, Bao XY, Lo YH, Wang D: ZnO nanowire UV photodetectors with high internal gain. Nano Letters 2007, 7: 1003–1009. 10.1021/nl070111xView Article
- Fan ZY, Wang DW, Chang PC, Tseng WY, Lu JG: ZnO nanowire field-effect transistor and oxygen sensing property. Applied Physics Letters 2004, 85: 5923–5925. 10.1063/1.1836870View Article
- Li QH, Liang YX, Wan Q, Wang TH: Oxygen sensing characteristics of individual ZnO nanowire transistors. Applied Physics Letters 2004, 85: 6389–6391. 10.1063/1.1840116View Article
- Heo YW, Tien LC, Norton DP, Kang BS, Ren F, Gila BP, Pearton SJ: Electrical transport properties of single ZnO nanorods. Applied Physics Letters 2004, 85: 2002–2004. 10.1063/1.1792373View Article
- Collins RJ, Thomas DG: Photoconduction and surface effects with zinc oxide crystals. Physical Review 1958, 112: 388–395. 10.1103/PhysRev.112.388View Article
- Mollow E: Proceedings of the conference on photoconductivity. New York: John Wiley and Sons, Inc; 1956.
- Studenikin SA, Golego N, Cocivera M: Carrier mobility and density contributions to photoconductivity transients in polycrystalline ZnO films. Journal of Applied Physics 2000, 87: 2413–2421. 10.1063/1.372194View Article
- Look DC, Reynolds DC, Litton CW, Jones RL, Eason DB, Cantwell G: Characterization of homoepitaxial p-type ZnO grown by molecular beam epitaxy. Applied Physics Letters 2002, 81: 1830–1832. 10.1063/1.1504875View Article
- Ueda K, Tabata H, Kawai T: Magnetic and electric properties of transition-metal-doped ZnO films. Applied Physics Letters 2001, 79: 988–990. 10.1063/1.1384478View Article
- Reynolds DC, Look DC, Jogai B, Litton CW, Collins TC, Harsch W, Cantwell G: Neutral-donor-bound-exciton complexes in ZnO crystals. Physical Review B 1998, 57: 12151–12155. 10.1103/PhysRevB.57.12151View Article
- Zimmler MA, Bao J, Capasso F, Muller S, Ronning C: Laser action in nanowires: observation of the transition from amplified spontaneous emission to laser oscillation. Applied Physics Letters 2008, 93: 3.View Article
- Bao JM, Zimmler MA, Capasso F, Wang XW, Ren ZF: Broadband ZnO single-nanowire light-emitting diode. Nano Letters 2006, 6: 1719–1722. 10.1021/nl061080tView Article
- Wang ZL, Song JH: Piezoelectric nanogenerators based on zinc oxide nanowire arrays. Science 2006, 312: 242–246. 10.1126/science.1124005View Article
- Banerjee D, Jo SH, Ren ZF: Enhanced field emission of ZnO nanowires. Advanced Materials 2004, 16: 2028–2032. 10.1002/adma.200400629View Article
- Keem K, Kim H, Kim GT, Lee JS, Min B, Cho K, Sung MY, Kim S: Photocurrent in ZnO nanowires grown from Au electrodes. Applied Physics Letters 2004, 84: 4376–4378. 10.1063/1.1756205View Article
- Shapira Y, Cox SM, Lichtman D: Chemisorption, photodesorption and conductivity measurements on ZnO surfaces. Surface Science 1976, 54: 43–59. 10.1016/0039-6028(76)90086-8View Article
- Cunningham J, Finn E, Samman N: Photo-assisted surface-reactions studied by dynamic mass-spectrometry. Faraday Discussions 1974, 58: 160.View Article
- Banerjee D, Lao JY, Wang DZ, Huang JY, Steeves D, Kimball B, Ren ZF: Synthesis and photoluminescence studies on ZnO nanowires. Nanotechnology 2004, 15: 404–409. 10.1088/0957-4484/15/3/029View Article
- Huang MH, Mao S, Feick H, Yan HQ, Wu YY, Kind H, Weber E, Russo R, Yang PD: Room-temperature ultraviolet nanowire nanolasers. Science 2001, 292: 1897–1899. 10.1126/science.1060367View Article
- Reynolds DC, Look DC, Jogai B, Hoelscher JE, Sherriff RE, Harris MT, Callahan MJ: Time-resolved photoluminescence lifetime measurements of the Gamma(5) and Gamma(6) free excitons in ZnO. Journal of Applied Physics 2000, 88: 2152–2153. 10.1063/1.1305546View Article
- Hirschwald WH: Zinc-oxide - an outstanding example of a binary compound semiconductor. Accounts of Chemical Research 1985, 18: 228–234. 10.1021/ar00116a001View Article
- Janotti A, Van de Walle CG: Oxygen vacancies in ZnO. Applied Physics Letters 2005, 87: 122102. 10.1063/1.2053360View Article
- Mosbacker HL, Strzhemechny YM, White BD, Smith PE, Look DC, Reynolds DC, Litton CW, Brillson LJ: Role of near-surface states in ohmic-Schottky conversion of Au contacts to ZnO. Applied Physics Letters 2005, 87: 012102. 10.1063/1.1984089View Article
- Vanheusden K, Warren WL, Seager CH, Tallant DR, Voigt JA, Gnade BE: Mechanisms behind green photoluminescence in ZnO phosphor powders. Journal of Applied Physics 1996, 79: 7983–7990. 10.1063/1.362349View Article
- Lagowski J, Sproles ES, Gatos HC: Quantitative study of charge-transfer in chemisorption - oxygen-chemisorption on ZnO. Journal of Applied Physics 1977, 48: 3566–3575. 10.1063/1.324156View Article
- Aphek OB, Kronik L, Leibovitch M, Shapira Y: Quantitative assessment of the photosaturation technique. Surface Science 1998, 409: 485–500. 10.1016/S0039-6028(98)00277-5View Article
- Fischer CH, Henglein A: Photochemistry of colloidal semiconductors. 31. Preparation and photolysis of CdS sols in organic-solvents. Journal of Physical Chemistry 1989, 93: 5578–5581. 10.1021/j100351a049View Article
- Korneeva AN, Vorontso ES: Thermodynamics and mechanism of carbo-thermal reduction of thin oxide-films on metals. Zhurnal Fizicheskoi Khimii 1972, 46: 1551.
- Suehiro J, Nakagawa N, Hidaka S, Ueda M, Imasaka K, Higashihata M, Okada T, Hara M: Dielectrophoretic fabrication and characterization of a ZnO nanowire-based UV photosensor. Nanotechnology 2006, 17: 2567–2573. 10.1088/0957-4484/17/10/021View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.